AWLGRIPTwo-Part Linear Polyurethane Enamel

Famous for its high gloss and chip-resistant durability, Awlgrip two-part polyurethane enamel provides resin-rich, clean, bright color. May be applied by brush, spray or roller when used with the appropriate converters. Awlgrip paints are lead-free and comply with Federal regulations. Recommended only for professional applicators using proper safety equipment.

NOTE: All Awlgrip products are two component products; they require a base (color) and a converter.

Base Formulation: Two-part aliphatic linear polyurethane

Recommended Application Method: Brush, roller or spray

Number of Coats Recommended: Spray: 2-3; Brush or roller: 2

Primer Needed: Spray: 545 Primer; Brush or roller: AwlQuick Primer

Drying Time to Recoat: Spray: 1-4hrs.; Brush or roller: At least 16hrs.

Drying Time to Full Cure: 14 days

Coverage: Spray: 530sq.ft./gal.; Brush or roller: 700-725 sq.ft/gal.

Converters/Reducers/Accelerators: Selected according to application method (brush or spray), ambient temperature and other factors

There are two converters: One for brush-H3002, and one for spray-G3010.

For spray applications, mixing Awlgrip is 1:1 base:converter (G3010). For brush applications, Awlgrip is mixed at the ratio of 2:1 (two parts base to 1 part converter (H3002). Both types of converters are listed below:

Famous for its high gloss and chip-resistant durability, Awlgrip two-part polyurethane enamel provides resin-rich, clean, bright color. May be applied by brush, spray or roller when used with the appropriate converters. Awlgrip paints are lead-free and comply with Federal regulations. Recommended only for professional applicators using proper safety equipment.

NOTE: All Awlgrip products are two component products; they require a base (color) and a converter.

Base Formulation: Two-part aliphatic linear polyurethane

Recommended Application Method: Brush, roller or spray

Number of Coats Recommended: Spray: 2-3; Brush or roller: 2

Primer Needed: Spray: 545 Primer; Brush or roller: AwlQuick Primer

Drying Time to Recoat: Spray: 1-4hrs.; Brush or roller: At least 16hrs.

Drying Time to Full Cure: 14 days

Coverage: Spray: 530sq.ft./gal.; Brush or roller: 700-725 sq.ft/gal.

Converters/Reducers/Accelerators: Selected according to application method (brush or spray), ambient temperature and other factors

There are two converters: One for brush-H3002, and one for spray-G3010.

For spray applications, mixing Awlgrip is 1:1 base:converter (G3010). For brush applications, Awlgrip is mixed at the ratio of 2:1 (two parts base to 1 part converter (H3002). Both types of converters are listed below:

Spray: 1 to 4 Hours; Brush or Roller: At Least 16 Hours to Overcoat; 14 Days to Full Cure

Type

Two-Part Aliphatic Linear Polyurethane

Capacity

Gallon

Color

Gray

Coverage

700 Square Feet

Cure Time

Spray: 1 to 4 Hours; Brush or Roller: At Least 16 Hours to Overcoat; 14 Days to Full Cure

Type

Two-Part Polyurethane

Capacity

Gallon

Color

Silver

Coverage

700 Square Feet

Cure Time

Spray: 1 to 4 Hours; Brush or Roller: At Least 16 Hours to Overcoat; 14 Days to Full Cure

Type

Two-Part Polyurethane

West Advisor

The West Advisor articles have answered boaters' questions and provided solutions to boating problems for more than 20 years. West Marine has compiled one of the Web's most comprehensive collections of technical boating information articles.